# T-criterion

﻿
T-criterion

The T-failure criterion [Andrianopoulos, N.P., Atkins, A.G., Experimental Determination of the Failure Parameters ΤD,0 and ΤV,0 in Mild Steels According to the T-criterion, ECF9 Reliability and Structural Integrity of Advanced Materials, Vol. III, 1992.] [Andrianopoulos, N.P., Metalforming Limit Diagrams According to the T-criterion, Journal of Materials Processing Technology 39, 1993.] is rather a set of failure criteria, that correlate the reversible elastic energy density storage process with both brittle and ductile failure. The development of this criterion is based on the unacceptable fact that pure hydrostatic loading of metals following the von Mises yield law, results in no failure, since the von Mises criterion is a function of deviatoric stresses. The strain energy density stored in the material and calculated by the area under the - curve represents the total amount of energy stored in the material only in the case of pure shear. In all other cases, there is a divergence between the actual and calculated stored energy in the material, which is maximum in the case of pure hydrostatic loading, where, according to the von Mises criterion, no energy is stored. This paradox is resolved if a second constitutive equation is introduced, that relates hydrostatic pressure p with the volume change $Theta$. These two curves, namely and (p-$Theta$) are essential for a complete description of material behaviour up to failure. Thus, two criteria must be accounted for when considering failure and two constitutive equations that describe material response. According to this criterion, an upper limit to allowable strains is set either by a critical value ΤV,0 of the elastic energy density due to volume change (dilatational energy) or by a critical value ΤD,0 of the elastic energy density due to change in shape (distortional energy). The volume of material is considered to have failed by extensive plastic flow when the distortional energy Τd reaches the critical value ΤD,0 or by extensive dilatation when the dilatational energy Τv reaches a critical value ΤV,0. The two critical values ΤD,0 and ΤV,0 are considered material constants independent of the shape of the volume of material considered and the induced loading, but dependent on the strain rate and temperature.

Deployment for Isotropic Metals

For the development of the criterion, a continuum mechanics approach is adopted. The material volume is considered to be a continuous medium with no particular form or manufacturing defect. It is also considered to behave as a linear elastic isotropically hardening material, where stresses and strains are related by the generalised Hook’s law and by the incremental theory of plasticity with the von Mises flow rule. For such materials, the following assumptions are considered to hold:
(a) The total increment of a strain component $depsilon_\left\{i,j\right\}$ is decomposed into the elastic and the plastic $depsilon_\left\{i,j\right\}^e$ increment and $depsilon_\left\{i,j\right\}^p$ respectively:
$depsilon_\left\{i,j\right\}=depsilon_\left\{i,j\right\}^e+depsilon_\left\{i,j\right\}^p$ (1)
(b) The elastic strain increment $depsilon_\left\{i,j\right\}^e$ is given by Hooke’s law:
$depsilon_\left\{i,j\right\}^e=cfrac\left\{1\right\}\left\{2G\right\}\left(d\left\{sigma\right\}_\left\{i,j\right\}-cfrac\left\{3 u\right\}\left\{1+\left\{ u\left\{delta\right\}_\left\{i,j\right\}dp\right)$(2)
where $G=cfrac\left\{E\right\}\left\{2\left(1+ u\right)\right\}$the shear modulus, $u$ the Poisson’s ratio and $\left\{delta\right\}_\left\{i,j\right\}$ the Krönecker delta.
(c) The plastic strain increment $depsilon_\left\{i,j\right\}^p$ is proportional to the respective deviatoric stress:
$depsilon_\left\{i,j\right\}^p=s_\left\{i,j\right\}d\left\{lambda\right\}$(3)
where $s_\left\{i,j\right\}=\left\{sigma\right\}_\left\{i,j\right\}-\left\{delta\right\}_\left\{i,j\right\}p$ and $d\left\{lambda\right\}$ an infinitesimal scalar. (3) implies that the plastic strain increment:
* depends on the value of stresses, not on their variation
* is independent of the hydrostatic component of the stress tensor
* is collinear with the deviatoric stresses (isotropic material)(d) The increment in plastic work per unit volume using (4.16) is:
$dw_\left\{p\right\}=\left\{sigma\right\}_\left\{i,j\right\}d\left\{epsilon\right\}_\left\{i,j\right\}^p=\left\{sigma\right\}_\left\{i,j\right\}depsilon_\left\{i,j\right\}d\left\{lambda\right\}$ (4)
and the increment in strain energy, $dT$, equals to the total differential of the potential $\left\{Pi\right\}$:
$dT=d\left\{Pi\right\}=pd\left\{Theta\right\}+\left\{sigma\right\}d\left\{epsilon\right\}=dT_\left\{V\right\}+dT_\left\{D\right\}^*$(5)
where$\left\{Theta\right\}=\left\{epsilon\right\}_\left\{11\right\}+\left\{epsilon\right\}_\left\{22\right\}+\left\{epsilon\right\}_\left\{33\right\}$, $p=cfrac\left\{1\right\}\left\{3\right\}\left\{sigma\right\}_\left\{11\right\}+\left\{sigma\right\}_\left\{22\right\}+\left\{sigma\right\}_\left\{33\right\}$ and for metals following the von Mises yield law, by definition
(6)
(7)
are the equivalent stress and strain respectively.In (5) the first term of the right hand side, $dT_\left\{V\right\}=pdTheta$ is the increment in elastic energy for unit volume change due to hydrostatic pressure. Its integral over a load path is the total amount of dilatational strain energy density stored in the material. The second term is the energy required for an infinitesimal distortion of the material. The integral of this quantity is the distortional strain energy density. The theory of plastic flow permits the evaluation of stresses, strains and strain energy densities along a path provided that $d\left\{lambda\right\}$ in (3) is known. In elasticity, linear or nonlinear, $d\left\{lambda\right\}$. In the case of strain hardening materials, $d\left\{lambda\right\}$ can be evaluated by recording the curve in a pure shear experiment. The hardening function after point “y” in Figure 1 is then:
(8)
and the infinitesimal scalar $d\left\{lambda\right\}$ is: (9)
where $dw_p\left(H\right)$is the infinitesimal increase in plastic work (see Figure 1). The elastic part of the total distortional strain energy density is:
(10)
where is the elastic part of the equivalent strain. When there is no nonlinear elastic behaviour, by integrating (4.22) the elastic distortional strain energy density is:
(11)
Similarly, by integrating the increment in elastic energy for unit volume change due to hydrostatic pressure, $dT_V=pdTheta$, the dilatational strain energy density is:
$T_V=int\left\{pdTheta\right\}=cfrac\left\{1\right\}\left\{2K\right\}p^2=cfrac\left\{1\right\}\left\{2\right\}K\left\{Theta\right\}^2$ (12)
assuming that the unit volume change $\left\{Theta\right\}$ is the elastic straining, proportional to the hydrostatic pressure, p (Figure 2):
$\left\{Theta\right\}=cfrac\left\{1\right\}\left\{2K\right\}p$ or $d\left\{Theta\right\}=cfrac\left\{1\right\}\left\{K\right\}dp$ (13)
where $\left\{Theta\right\}=\left\{epsilon\right\}_\left\{11\right\}+\left\{epsilon\right\}_\left\{22\right\}+\left\{epsilon\right\}_\left\{33\right\}$, $p=cfrac\left\{1\right\}\left\{3\right\}\left\{sigma\right\}_\left\{11\right\}+\left\{sigma\right\}_\left\{22\right\}+\left\{sigma\right\}_\left\{33\right\}$ and $K=cfrac\left\{E\right\}\left\{3\left(1-2 u\right)\right\}$ the bulk modulus of the material.
In summary, in order to use (12) and (13) to determine the failure of a material volume, the following assumptions hold:
* The material is isotropic and follows the von Mises yield condition
* The elastic part of the stress-strain curve is linear
* The relationship between hydrostatic pressure and unit volume change is linear
* The derivative (hardening slope) must be positive or zero

Limitations

The criterion will not predict any failure due to distortion for elastic-perfectly plastic, rigid-plastic, or strain softening materials. For the case of nonlinear elasticity, appropriate calculations for the integrals in and (12) and (13) accounting for the nonlinear elastic material properties must be performed. The two threshold values for the elastic strain energy $T_\left\{V,0\right\}$ and $T_\left\{D,0\right\}$ are derived from experimental data. A drawback of the criterion is that elastic strain energy densities are small and comparatively hard to derive. Nevertheless, example values are presented in the literature as well as applications where the T-criterion appears to perform quite well.

References

Wikimedia Foundation. 2010.

### Look at other dictionaries:

• Criterion Games — Type Subsidiary of Electronic Arts Industry Video game industry Founded 1993 Headquarters …   Wikipedia

• Criterion — may refer to: Criterion, general meaning In science and mathematics: Criterion validity, in psychometrics, a measure of how well one variable or set of variables predicts an outcome Criterion referenced test, translates a test score into a… …   Wikipedia

• Criterion Games — Тип Дочернее общество Год основания 1993 Расположение …   Википедия

• Criterion of embarrassment — Criterion of embarrassment: The Baptism of Jesus The criterion of embarrassment, also known as criterion of dissimilarity, is a critical analysis of historical accounts in which accounts embarrassing to the author are presumed to be true because… …   Wikipedia

• Criterion of multiple attestation — Criterion of multiple attestation: Last Supper The criterion of multiple attestation or independent attestation is a tool used by Biblical scholars to help determine whether certain actions or sayings by Jesus in the New Testament are from… …   Wikipedia

• Criterion Place — General information Status Never built Location Sovereign Street, Leeds, England Construction started 2008 Estimated completion …   Wikipedia

• Criterion Theatre (Coventry) — Criterion Theatre Address Berkeley Road South Earlsdon City Coventry West Midlands …   Wikipedia

• Criterion Software — Criterion Games Criterion Games Dates clés 1993 Fondation 2004 Rachat par EA …   Wikipédia en Français

• Criterion Hotel Perth (Perth) — Criterion Hotel Perth country: Australia, city: Perth (City) Criterion Hotel Perth The Criterion Hotel Perth is the newest hotel open in June 1996. Situated in the heart of the business district, it is just minutes walk to key commercial… …   International hotels

• Criterion Properties plc v Stratford UK Properties LLC — Criterion plc v Stratford LLC Court House of Lords Full case name Criterion Properties plc v Stratford UK Properties LLC Citation(s)  UKHL 28 Case history …   Wikipedia

• Criterion Theatre (disambiguation) — Criterion Theatre or Criterion Theater may refer to: in Australia Criterion Theatre (Sydney), a demolished theatre in Sydney, Australia in England Criterion Theatre, a theatre situated on Piccadilly Circus, London, England Criterion Theatre… …   Wikipedia

We are using cookies for the best presentation of our site. Continuing to use this site, you agree with this.